CEMENT CONCRETE MIX DESIGNDr.K.Lakshmi pathiCentre Head CRIMAMR-APARD
DEFINITION The process of selecting suitable ingredients of concrete and determining their relative quantities with the objective of producing a concrete of the required strength, durability, and workability as economically as possible, is termed the concrete mix design
Nominal Mixes In the past the specifications for concrete prescribed the proportions of cement, fine and coarse aggregates. These mixes of fixed cement-aggregate ratio which ensures adequate strength are termed nominal mixes. These offer simplicity and under normal circumstances, have a margin of strength above that specified. However, due to the variability of mix ingredients the nominal concrete for a given workability varies widely in strengthTypes of Mixes
Nominal mix concreteTraditional way of mix proportion specified in terms of fixed ratios of Cement : Sand : coarse aggregate (In general by volume)*C502.5Useful for small works
Useful for routine concrete construction
Limited up to M20 grade
Requires high cement content
The nominal mixes of fixed cement-aggregate ratio (by volume) vary widely in strength and may result in under- or over-rich mixes. For this reason, the minimum compressive strength has been included in many specifications. These mixes are termed standard mixes.Standard mixes
IS 456-2000 has designated the concrete mixes into a number of grades as M10, M15, M20, M25, M30, M35 and M40. In this designation the letter M refers to the mix and the number to the specified 28 day cube strength of mix in N/mm2. The mixes of grades M10, M15, M20 and M25 correspond approximately to the mix proportions (1:3:6), (1:2:4), (1:1.5:3) and (1:1:2) respectively.
The proportions generally adopted are as given below
Grade of ConcreteNominal Mix proportions (Cement: FA : CA) M 51:5:10M7.51:4:8M101:3:6M151:2:4M201:1.5:3
In these mixes the performance of the concrete is specified by the designer but the mix proportions are determined by the producer of concrete, except that the minimum cement content can be laid down. This is most rational approach to the selection of mix proportions with specific materials in mind possessing more or less unique characteristics.
Several methods of mix design evolved over the years in different countries
Ex: ACI practice, British practice, Indian Standard recommendations. etc.
DESIGN MIX CONCRETE
RECOMMENDATIONS FOR CONCRETE MIX DESIGN ARE GIVEN IN
I.S.10262-1982 & I.S.10262-2009
Designed mix should meet the design requirements in the fresh and hardened states
FACTORS AFFECTING THE CHOICE OF MIX PROPORTIONSThe various factors affecting the mix design are:1. Compressive strengthIt is one of the most important properties of concrete and influences many other describable properties of the hardened concrete. The mean compressive strength required at a specific age, usually 28 days, determines the nominal water-cement ratio of the mix. The other factor affecting the strength of concrete at a given age and cured at a prescribed temperature is the degree of compaction. According to Abrahams law the strength of fully compacted concrete is inversely proportional to the water-cement ratio.
2. WorkabilityThe degree of workability required depends on three factors. These are the size of the section to be concreted, the amount of reinforcement, and the method of compaction to be used. For the narrow and complicated section with numerous corners or inaccessible parts, the concrete must have a high workability so that full compaction can be achieved with a reasonable amount of effort. This also applies to the embedded steel sections. The desired workability depends on the compacting equipment available at the site.
3. DurabilityThe durability of concrete is its resistance to the aggressive environmental conditions. High strength concrete is generally more durable than low strength concrete. In the situations when the high strength is not necessary but the conditions of exposure are such that high durability is vital, the durability requirement will determine the water-cement ratio to be used.
4. Maximum nominal size of aggregateIn general, larger the maximum size of aggregate, smaller is the cement requirement for a particular water-cement ratio, because the workability of concrete increases with increase in maximum size of the aggregate. However, the compressive strength tends to increase with the decrease in size of aggregate.IS 456:2000 and IS 1343:1980 recommend that the nominal size of the aggregate should be as large as possible.
5. GRADING AND TYPE OF AGGREGATE
The grading of aggregate influences the mix proportions for a specified workability and water-cement ratio. Coarser the grading leaner will be mix which can be used. Very lean mix is not desirable since it does not contain enough finer material to make the concrete cohesive.
The type of aggregate influences strongly the aggregate-cement ratio for the desired workability and stipulated water cement ratio. An important feature of a satisfactory aggregate is the uniformity of the grading which can be achieved by mixing different size fractions.
6. QUALITY CONTROL
The degree of control can be estimated statistically by the variations in test results. The variation in strength results from the variations in the properties of the mix ingredients and lack of control of accuracy in batching, mixing, placing, curing and testing. The lower the difference between the mean and minimum strengths of the mix lower will be the cement-content required. The factor controlling this difference is termed as quality control.
MIX PROPORTION DESIGNATIONS
The common method of expressing the proportions of ingredients of a concrete mix is in the terms of parts or ratios of cement, fine and coarse aggregates. For e.g., a concrete mix of proportions 1:2:4 means that cement, fine and coarse aggregate are in the ratio 1:2:4 or the mix contains one part of cement, two parts of fine aggregate and four parts of coarse aggregate. The proportions are either by volume or by mass. The water-cement ratio is usually expressed in mass
FACTORS TO BE CONSIDERED FOR MIX DESIGN
The grade designation giving the characteristic strength requirement of concrete.The type of cement influences the rate of development of compressive strength of concrete.Maximum nominal size of aggregates to be used in concrete may be as large as possible within the limits prescribed by IS 456:2000.The cement content is to be limited from shrinkage, cracking and creep.The workability of concrete for satisfactory placing and compaction is related to the size and shape of section, quantity and spacing of reinforcement and technique used for transportation, placing and compaction.
I S CODE METHOD OF MIX DESIGN*C502.6
Target strength for mean strength The target mean compressive strength at 28 days (ft) =fck+ K.S
K = a statistical value , usually taken as 1.65 S = standard deviation for each grade of concrete ( table 8 of I.S. 456 -2000 )
* Values of K
Accepted proportion of low resultsK1 in 5, 20%0.841 in 10, 10%1.281 in 15, 6.7%1.501 in 20, 5%1.651in 40, 2.5%1.861 in 100, 1%2.33
TABLE-8, IS CODEC502.6*
Grade of concreteAssumed Standard ,Deviations (N/mm )M 10 ,M 153.5M 20, M254.0M 30, M 35, M 40, M 45 & M 505.0
C502.6*A) The free water cement ratio corresponding to the target strength is to be determined from the graph shown in fig.2.Selection of water cement ratio :
Modified graph for Selection of water cement ratio :
B) The water cement ratio, as selected above should be checked against the limiting water cement ratio for the durability requirements as given in table
ExposurePlain ConcreteReinforced ConcreteMin.CementMaxw/cMingradeMin.CementMaxw/cMingradeMild220kg/m30.60--300kg/m3
0.55M 20Moderate240kg/m30.60M 15300kg/m30.50M 25Severe250kg/m30.50M 20320kg/m30.45M 30V. Severe260kg/m30.45M 20340kg/m30.45M 35Extreme280kg/m30.40M 25360kg/m30.40M 40
Durability Criteria as per IS 456- 2000Adjustments to minimum cement content for aggregates other than 20 mm nominal max. size aggregates as per IS 456: 2000.
10 mm+ 40 kg/cum20 mm040 mm- 30 kg/cum
PlacingconditionDegreeSlump(mm)CompactionfactorMass concrete, lightly reinforced sections in beams, walls, columns and floorsLOW25 to 750.8 to 0.85Heavily reinforced sections in slabs, beams, walls, columns and footingsMEDIUM50 to 1000.9 to 0.92Slip formwork, pumped concrete, in- situ pilingHIGH100 to 1500.95 to 0.96
* Approximate water content (Kg) per cubic metre of concrete (Table 32, SP:23-1982)
Slump(mm)Maximum Size of Aggregate(mm)10204030-5020518516080-100225200175150-180240210185
3.Estimation of entrapped air
Depends on nominal max size of aggregate as given in table
Max. size of aggregate (mm)Entrapped air as % of volume of concrete 103.0202.0401.0
4. Selection of water content and fine to total aggregate ratio
The values are given in the tables, based on the following conditions
(a) Crushed (Angular) Coarse aggregate conforming to IS: 383(b) Sand conforming to grading zone II of table 4 of IS 383(c) Workability corresponds to C.F. of 0.8*C502.6
5.a. Approximate sand and water contents per cu.m of concrete W/C = 0.6, Workability = 0.8 C.F. (For medium strength concrete up to M35)C502.6*
Maximum size of aggregate (mm)Water content including surface water per m of concrete (kg)Sand as % of total aggregate by absolute volume102004020186354016530
Step 5 - Estimation of Coarse Aggregate Proportion For W/C ratio of 0.5 use following Table
Correction in Coarse Aggregate values The table specified for W/C ratio of 0.51. For Every +0.05 change in W/C ratio: -0.012. For Every -0.05 change in W/C ratio: +0.013. For Pumpable Mix : -10 %57
5.c. Adjustments of values in Water Content and sand % for other conditionsC502.6*
Change in conditions stipulated for tablesAdjustment required in Water contents % sand in total aggregateFor sand conforming to zone I ,zone III or zone Iv of I.S 383-1979 0+1.5%for zone I-1.5% for zone III-3.0 % for zone IvIncrease or decrease in the value of compacting factor by 0.1 3% 0
Each 0.05 increase or decrease in water cement ratio 0 1.0 %For rounded aggregates-15kg/m -7 %
For Other Conditions as per IS:10262,2009
ConditionCorrectionSub-Angular Aggregates- 10 KgGravel + Crushed Particles- 20 KgRounded Gravel- 25 KgFor every slump increase of 25 mm+ 3 %Use of Water Reducing Admixture- 5 to 10 %Use of Superplasticzing Admixtures- 20 %54
6.Determination of cement content
a) From free W/C ratio and b) quantity water per unit volume of concrete for workability (as derived in 5.c) Cement by mass = (Water content) / (w.c.r.)
This cement content should not be less than minimum content from the aspect of durability (given in 2.b)
7.Calculation of aggregate content (fa and Ca)
where V = absolute volume of concrete= gross volume (1m3) minus the volume of entrapped airSc = specific gravity of cementW = Mass of water per cubic metre of concrete, kgC = mass of cement per cubic metre of concrete, kgp = ratio of fine aggregate to total aggregate by absolute volumefa, Ca = total masses of fine and coarse aggregates, per cubic metre of concrete, respectively, kg, andSfa, Sca = specific gravities of saturated surface dry fine and coarse aggregates, respectively
9. Determine the concrete mix proportions for the first trial mix.10. Prepare the concrete using the calculated proportions and cast three cubes of 150 mm size and test them wet after 28-days moist curing and check for the strength.11. Prepare trial mixes with suitable adjustments till the final mix proportions are arrived at.
*So the mix proportion works out to be
W : C : fa : ca = 185 : 411 : 635 : 1150= 0.45 : 1 : 1.55 : 2.80
This mix will be considered as Trial Mix No.2
*Step VII:- Make slump trials to find out the actual weight of water to get required slump. Make corrections to the water content & %FA, if required.
Step VIII:- Compute 2 more trial mixes with W/C ratios as 0.40 & 0.50, taking %FA as 34% and 38% respectively.
*Trial Mix No. 1:-Cement = 185 / 0.4 = 462.5 Kg.Substituting the values in Eq(1), we get1000 = 185 + 462.5/3.0 + (1/0.34) * fa /2.6)fa = 584 Kg. Substituting the values in Eq(2), we get1000 = 185 + 462.5/3.0 + (1/0.66) * ca /2.65)ca = 1156 Kg. So the mix proportion works out to beW : C : fa : ca = 185 : 462.5 : 584 : 1156= 0.4 : 1 : 1.26 : 2.50
*Trial Mix No. 3:-Cement = 185 / 0.5 = 370 Kg.Substituting the values in Eq(1), we get1000 = 185 + 370/3.0 + (1/0.38) * fa /2.6)fa = 683 Kg. Substituting the values in Eq(2), we get1000 = 185 + 370/3.0 + (1/0.62) * ca /2.65)ca = 1136 Kg. So the mix proportion works out to beW : C : fa : ca = 185 : 370 : 683 : 1136= 0.5 : 1 : 1.85 : 3.07
Step IX:- Cast atleast 3 cubes for each trial mix.
Step X:- Test the cubes for compressive strength at 28 days.
*28 Days Compressive Strengths of Trial Mixes
W/C RatioC/W RatioCompressive Strength (Kg/Cm2)0.402.504570.452.224200.502.00360
Step XI:- Draw a graph between compressive strength Vs C/W Ratio.
Step XII:- From the graph, find the W/C ratio for the required target mean compressive strength.
Step XIII:- Calculate the mix proportions corresponding to the W/C ratio, obtained from the graph.
*Final Mix:-From the graph, for a target strength of 390 Kg/Cm2, W/C ratio = 0.47Cement = 185 / 0.47 = 394 Kg.Substituting the values in Eq(1), we get1000 = 185 + 394/3.0 + (1/0.38) * fa /2.6)fa = 675 Kg. Substituting the values in Eq(2), we get1000 = 185 + 394/3.0 + (1/0.62) * ca /2.65)ca = 1123 Kg. So the mix proportion works out to beW : C : fa : ca = 185 : 394 : 675 : 1123= 0.47 : 1 : 1.71 : 2.85
*Step XIV:- Check the cement content & W/C ratio against the limiting values given in Table-5 of I.S: 456-2000 for given type of exposure & type of Concrete.
*Table-5 Minimum Cement content Maximum Water-Cement ratio and Minimum Grade of Concrete for different exposures with normal weight of aggregate of 20mm nominal maximum size.
ExposurePlain ConcreteReinforced ConcreteMinimum Cement Content kg/m3Maximum Free Water Cement RatioMinimum Grade of ConcreteMinimum Cement Content kg/m3Maximum Free Water Cement RatioMinimum Grade of Concretei)Mild2200.60-3000.55M20ii)Moderate2400.60M153000.50M25iii)Severe2500.50M203200.45M30iv)Very Severe2600.45M203400.45M35v)Extreme2800.40M253600.40M40
*From the table 5 of IS: 4562000, the minimum Cement content & W/C ratio, For moderate, for RCC are 300Kgs. & 0.5
The Cement content = 394Kgs. > 300Kgs. Hence Ok
The W/C Ratio = 0.47 < 0.5 Hence Ok
* TEST REPORTConcrete Mix RCC M30 with 20.0mm M.S.A.
Sl.No.ParticularsResult1Characteristic Compressive strength in N/Sq.mm302Maximum size of Aggregate in mm20.03Type of ExposureModerate4Type of Site controlGood5Target Average Compressive Strength in N/Sq.mm38.26Workability in terms of Slump in mm25-757Mode of CompactionVibration8Mix Partiuclars:a.Water-Cement Ratiob.Materials per cubic metre of concrete in Kg.i)Waterii)Cement (OPC 43 Grade)iii)Fine Aggregateiv)Coarse Aggregatec.Mix Portion by weight 0.47
CONVERTING WEIGHT TO VOLUME Unit weight of Cement =1440 Kg/mt3
Unit weight of F.A =1600 Kg/mt3
Unit weight of C.A =2200 Kg/mt3
1 bag of cement =1.25 cft
Proportions for Nominal Mix Concrete
Grade of ConcreteTotal qty of dry aggregate (CA + FA) per 50 kg cementProportion of FA to CA by volumeWater per 50 kg cement (max) litM 58001: 2 (Zone II) subject to upper limit of 1: 1.5 (Zone I)& lower limit of 1: 2.5 (ZoneIII)60M 7.562545M 1048034M 1533032M 202503064
Example for Nominal Mixes Grade of Concrete: M 20 Total Aggregate (CA + FA) per 50 kg cement: 250 kg, FA of Zone II (say) Water content: 30 lit per 50 kg cement w/c ratio= 30/50= 0.60 Considering FA: CA= 1: 2, Sand= (250 X 1)/ 3= 83 kg Coarse Aggregate= (250 X 2)/ 3= 167 kg65
CementFACAWater50 kg (35 Lit)83 kg167 kg30 lit
Major Changes in : IS 10262
S,NOld Edition 1982Revised 2009 Edition1Title - " Recommanded guidelines for Concrete mix Desiqn11Title - "Concrete mix Proportioning - Guidelines12Applicability was not specified for any specific Concrete GradesSpecified for Ordinary (M 10 - M 20} and Standard (M25 - M 55) Concrete Grades only.3Based on IS 456 : 1982Modification in iine with IS 456 : 20004W / C ratio was based on Concrete grade and 28 days compressive strength of Concrete and the durability criteriaW/C ratio is based on Durability criteria and the Experience and Practical trials5Water Content could be modified taking into account the compaction factor value (Laboratory based test for Workability) and the shape of aggregates.Water content can be modified Based on Slump vale (Field test of Workability) and Shape of Aggreagtes, and use of Admixtu res.6Entrapped Air cotent considered according to Nominal Maximum size of AggregatesNo Entrapped Air content taken into account7Not much Consideration for Trial MixesTrial Mixes concept is mentionedeConcrete Mix Design with Fly ash is not mentionedAn illustrative example of Concrete Mix Prportioning using Fly ash has been added
M 20 Grade Concrete (by Volume) is 1: 1.5 % : 366
CementFACAWater50 kg83 kg167 kg30 lit(by weight) 11.663.320.61.43 kg/ lit1.52 kg/ lit1.60 kg/ lit35 lit54.6 lit104.4 lit30 lit(by volume) 11.562.98
Click here to load reader